## Dynamics of vortex fronts

## in type II superconductors

## Dynamics of vortex fronts

## in type II superconductors

proefschrift

ter verkrijging van

de graad van Doctor aan de Universiteit Leiden,

op gezag van de Rector Magnificus Dr. D. D. Breimer,

hoogleraar in de faculteit der Wiskunde en

Natuurwetenschappen en die der Geneeskunde,

volgens besluit van het College voor Promoties

te verdedigen op dinsdag 22 November 2005

te klokke 14.15 uur

door

### Chiara Baggio

Overige leden: Prof. dr. J. Aarts

Prof. dr. A. Ach´ucarro

Prof. dr. C. W. J. Beenakker

**Contents**

**1** **Introduction** **1**

1.1 Perspective . . . 1

1.2 Ginzburg-Landau and London theories . . . 6

1.3 Type II superconductors . . . 10

1.4 Magnetic properties of vortices . . . 13

1.4.1 Magnetic ﬁeld of a ﬂux line . . . 14

1.4.2 Vortex-line Energy . . . 15

1.4.3 Interaction between vortices . . . 16

1.4.4 Interactions in a thin ﬁlm . . . 17

1.5 The Lorentz force . . . 17

1.6 The dynamics of vortices . . . 19

1.6.1 The ﬂux ﬂow regime . . . 21

1.6.2 The creep regime . . . 22

1.7 Thermomagnetic instabilities . . . 25

1.8 Out-of-equilibrium vortex patterns . . . 29

**2** **Finger-like patterns** **35**
2.1 The sharp interface limit . . . 35

2.2 The model . . . 39

2.2.1 The physical background and the geometry . . . 39

2.2.2 Basic equations for the front dynamics . . . 40

2.2.3 Interfacial formulation . . . 42

2.3 Solution for the sharp E-j characteristic . . . 46

2.3.1 Derivation of the equation . . . 46

2.3.2 Results . . . 49

2.4 Solution for the smooth E-j characteristic . . . 53

2.4.1 Derivation of the equation . . . 53

2.4.2 Results . . . 56

2.5 Conclusions . . . 59

**3** **Vortex-antivortex front** **63**
3.1 Introduction . . . 63

3.1.1 Motivation . . . 63

3.1.2 The model . . . 68

3.1.3 Outline . . . 72

3.2 The planar front . . . 73

3.2.1 The equations and boundary conditions . . . 73

3.2.2 Singular behavior of the fronts . . . 75

3.2.3 Planar front proﬁle . . . 79

3.3 Dynamics in the presence of anisotropy . . . 81

3.3.1 Dynamical equations . . . 81

3.3.2 The linear stability analysis . . . 82

3.3.3 The shooting method . . . 84

3.3.4 Results . . . 89

3.4 Stationary front . . . 91

3.5 Conclusions . . . 95

**4** **Concluding remarks** **97**
4.1 Finger-like patterns. . . 99

4.1.1 Contour dynamics . . . 100

4.1.2 Preliminary results of the simulations . . . 102

4.2 Stability of a vortex-antivortex front . . . 104

*Contents*

**Bibliography** **111**

**Samenvatting** **117**

**Curriculum vitæ** **121**

**Chapter 1**

**Introduction**

**1.1**

**Perspective**

Superconductors are materials characterized not only by a perfect

conduc-tance below a critical temperature, as was ﬁrst discovered by Kamerlingh

Onnes in 1911 in Leiden, but also by the diamagnetic property of expelling an

external magnetic ﬁeld, the so called Meissner-Ochsenfeld eﬀect [1]. In type II

superconductors for external ﬁelds between the two temperature-dependent

values *H _{c}*

_{1}and

*H*

_{c}_{2}, ﬂux penetration occurs in the form of quantized ﬂux lines or vortices, with a quantum ﬂux

*φ*

_{0}=

*hc/2e*[2]. These are elastic and interacting objects, whose fascinating physics has attracted many scientists

in the last decades. After the discovery of the high-T* _{c}* superconductors, the
richness of the phenomenology of vortices, both in their static and

dynam-ical properties, has led to the introduction of the new concept of “vortex

matter” as a new state of matter [3]. From the technological point of view,

the intense research activity on type II superconductors was also stimulated

and motivated by the fact that, when vortices move they induce dissipation,

due to the normal nature of the cores, and therefore the superconducting

property of perfect conductivity is lost.

The properties of type II superconductors have been studied extensively

### a)

_{b)}

Figure 1.1: Examples of vortex patterns in type II superconductors. a) On

the left dendritic patterns of vortices with branchlike structures in a Nb ﬁlm

of 0.5*μm. The sample is at a temperature of 5.97 K and the external ﬁeld is*
135 Oe. After [10]. b) On the right droplet-like patterns observed with the

decoration technique in a NbSe_{2} single crystal at 5 mT. Inside the droplet

the density of vortices is higher, whereas in the outer region, where vortices

are more visible, the density is lower. After [17, 18].

rise to a rich variety of phases whose main features are by now rather well

understood [3–6]. In comparison with the equilibrium state, however, our

un-derstanding of the dynamics of vortices, and, in particular, of their collective

behavior is less well developed.

Recently, experiments with magneto-optical techniques on ﬂux

penetra-tion in thin ﬁlms have revealed the formapenetra-tion of a wide variety of instabilities.

When vortices penetrate from the edge of a superconductor, the pinning, due

to material imperfections, leads, in a idealised situation, to a ﬂux gradient

and thus to a linear proﬁle for the magnetic induction inside the sample.

This state (corresponding to the conventional picture of a so-called Bean

state [7]), is only marginally stable. In reality, ﬂux penetration can occur

in the form of a more complex distribution. Beyond phenomena such as

*interest-1.1. Perspective*

Figure 1.2: Images of ﬂux penetration (bright areas) into a superconducting

state (dark areas) at 5 K in a MgB_{2} ﬁlm of 0.4 *μm. From a) to d): images*
taken at an applied ﬁeld of 3.4 mT, 8.5 mT, 17 mT, and 60 mT, respectively.

From e) to f) Images taken at 21 mT and 0 mT during the ﬁeld reduction.

The one-dimensional structures of vortices at the initial stage develop into

dendritic patterns with a more complex morphology. After [11].

ing out-of-equilibrium patterns involving the formation of ramiﬁed dendritic

or ﬁnger-shaped domains of vortices, both in low-T* _{c}* materials, like in Nb and
MgB

_{2}thin ﬁlms [10–15], and high-T

*materials, like YBa*

_{c}_{2}Cu

_{3}O

_{7}

*[16]. Ex-amples of patterns presenting the morphology of dendrites, are represented in*

_{−}_{δ}Fig. 1.1(a) and Fig. 1.2 [10,17,18]. Figure 1.1(a), which refers to experiments

performed with magneto-optical techniques in a Nb thin ﬁlm, represents the

magnetic ﬂux distribution of the sample at a temperature of 5.97 K; the

brightness corresponds to the diﬀerent density of magnetic ﬂux. The same

type of patterns could be reproduced in MgB_{2}, as one can see in Fig. 1.2,

for diﬀerent magnetic ﬁelds. At lower temperatures the magnetic ﬂux

pene-trates instead through the nucleation of one-dimensional structures (ﬁngers

of vortices) that propagate with a very well deﬁned shape as we will show

later in this Chapter, in Sec. 1.8.

ex-tremely fast and are found only in a certain temperature window, are

in-stabilities of thermo-magnetic origin, due to the local overheating induced

by the vortex dynamics, but properties like their characteristic shape or the

velocity of propagation are still poorly understood [8, 9, 19–21].

Likewise, ﬂux penetration in the form of droplets have been observed in

NbSe_{2} single crystals [17, 18]. Figure 1.1(b) illustrates a droplet-like pattern

with a higher density of vortices inside and a lower density in the region

outside, where individual vortices are more visible. One can notice the high

degree of order of the vortex lattice inside the droplet and the sharp transition

zone between the two regions of vortices.

Furthermore, an other type of instability was observed at the boundaries

between ﬂux and anti-ﬂux in YBa_{2}Cu_{3}O_{7}* _{−}_{δ}*samples. By applying an external
ﬁeld of opposite sign to a remanent state, for a certain temperature interval,

the front between vortices and antivortices exhibits a “turbulent” behavior

[22–25], as we will see at the end of this Chapter. The mechanism that

underlies this phenomenon has been object of dicussions in the literature;

from this debate, the question about the relevance of the coupling of the

vortex mobility with the temperature for the instability has emerged [26–28].

Several attempts to describe the phenomenon have been made, but there are

still open issues to investigate in order to give a clear picture of such a

behavior.

A ﬁrst question on all these out-of-equilibrium patterns in type II

su-perconductors is which is the mechanism that generates the instability and

leads to the ﬁnal distribution of nonuniform magnetic ﬂux. Moreover, a

second issue is understanding the features of these structures, like their

char-acteristic shape and size. In this thesis we will focus on these topics, by

addressing two examples of propagating fronts between phases of diﬀerent

densities of vortices. As we will discuss, these types of phenomena present

analogies with interfacial instabilities in other physical systems like, for

ex-ample, dendrites in crystal growth or ﬁngering at the interface between two

*1.1. Perspective*

for the case of superconductor-normal interfaces in type I superconductors,

but the connection between these patterns and the ones observed in type

II superconductors has not been explored in depth. This is partly because

dealing with this analogy turns out to be a quite delicate issue. Firstly, the

systems with which we deal are strongly out-of-equilibrium, due to the

repul-sive long-range interactions between the ﬂux lines, expecially in thin ﬁlms;

thus equilibrium properties, like the surface tension at the interface between

two states, are not properly deﬁned. Secondly, systems of vortices are

char-acterised by properties which are not standard: their dynamics is strongly

nonlinear, and temperature dependent, and, moreover, inhomogeneities due

to pinning defects and temperature ﬂuctuations play an important role.

On the other hand, some techniques that are usually employed in the

analysis of front propagation are useful tools to investigate these instabilities,

like, for example, the description of the interface between two phases as a

sharp transition zone. In our work, we will study some patterns in type II

superconductors, by combining the ideas derived from the general perspective

of a pattern formation background with the theory of vortex dynamics. This

analysis requires also accommodating the description of the contour dynamics

of a domain of vortices, into a macroscopic picture, where the density of

vortices is a continuum coarse-grained ﬁeld.

This thesis has the following structure. The remaining part of this

chap-ter introduces basic concepts on superconductivity and vortex patchap-terns to

give the reader the necessary background for the comprehension of this work

and to oﬀer a general view on the types of dynamical instabilities that we will

analyse. We will ﬁrst start from a brief description of the phenomenological

Ginzburg-Landau and London theories; then we will deﬁne type II

super-conductors and the quantised ﬂuxoid. The properties of Abrikosov vortices,

like the energy of interaction for a slab and a ﬁlm will then be discussed.

Since in this thesis we are interested mainly in the dynamics of vortices and

their collective behavior, we will focus thereafter on the dynamical regimes of

on the thermo-magnetic instabilities that are observed in the intermediate

state by presenting some examples of patterns in type II superconductors

regarding some recent experiments.

In Chapter 2 we will deal with ﬁnger-like patterns in Nb [13, 14]. We will

analyse these instabilities by building a model that takes into account the

coupling with the local temperature of the sample and formulate a novel type

of approach based on a sharp interface description. The main purpose of this

study is to derive features like the well deﬁned ﬁnger shape, the width and

their dependence with the substrate temperature. This theoretical model is

the ﬁrst example that clearly exhibits this type of ﬁngered-shape patterns.

In Chapter 3, instead, we will examine the dynamics of a front between

ﬂux and anti-ﬂux in the presence of an in-plane anisotropy. In this work

we aim to understand the origin of the turbulence that was observed at the

boundaries between regions with vortices and antivortices in YBa_{2}Cu_{3}O_{7}* _{−}_{δ}*,
that we have mentioned above [24].

Finally, in Chapter 4 we will summarize the main ideas and add some

remarks on the dynamics of vortex fronts which are discussed in the previous

chapters.

**1.2**

**Ginzburg-Landau and London theories**

The Ginzburg-Landau theory provides a very eﬀective tool for a

phenomeno-logical description of the properties of vortices [4, 5, 32]. Also within the

general perspective of the theory of front propagation, the Ginzburg-Landau

equations are often used to analyse the formation of patterns. In particular,

in the study of pattern-forming systems, like e.g. in the Rayleigh-B´enard

con-vection, the Ginzburg-Landau equations are studied in the form of amplitude

equations for traveling waves [33,34]. Within the framework of the more

spe-ciﬁc problem of front propagation in superconductors, the Ginzburg-Landau

equations provide a phenomenological method to analyse the dynamics and

*1.2. Ginzburg-Landau and London theories*

This approach has generally restricted to type I superconductors [35–38],

whereas for type II superconductors only few cases in the literature are

en-countered [39].

While the surface energy at the interface between the normal and

su-perconducting states in a type I superconductor is positive, for a type II

superconductor this is negative; therefore normal domains are unstable and

subdivide until this process is limited by a microscopic length *ξ, determined*
by the balance of the tendency to break up and the penalty of having too

rapid variations in the superconducting properties.

Therefore, the reason why the Ginzburg-Landau method is not so directly

used for a description of patterns in type II superconductors is that one needs

to go beyond the microscopic scale*ξ*and adopt a more macroscopic approach,
where the density of vortices is a continuum coarse-grained ﬁeld.

In order to present the basic concepts to understand this thesis, we will

here summarise brieﬂy the main points of this formalism.

The Ginzburg-Landau theory is based on the postulate that the free

en-ergy functional *F* for the superconducting state can be expressed through

an expansion of the complex order parameter *ψ(***r**) =*|ψ(***r**)*|*exp(iϕ(**r**)), that
is assumed to be small near the critical temperature *T _{c}* and vary slowly in
space. This functional is derived by imposing that it must be analytical and

real, as

*F* =

*d***r**

*α|ψ|*2+*β*
2*|ψ|*

4_{+} 1

2m*∗*

_{i}∇ −e∗*c* **A**

*ψ*

2

+(*∇ ×***A**)

2

8π

*,* (1.1)

where**A**is the vector potential of the microscopic magnetic ﬁeld**h**=*∇×***A**.

Here the ﬁelds are measured in Gaussian units. The eﬀective charge is given

by *e∗* = 2e, according to the BCS [40] microscopic theory of Cooper pairs,
while for the eﬀective mass*m∗* we assume the value*m∗* = 2m, where*m*is the
mass of the electron. From equation (1.1) in the absence of magnetic ﬁelds,

one can easily see that the constant coeﬃcient*β* must be positive, otherwise
the free energy would not be bounded from below. Moreover, depending on

(α >0) or at

*|ψ|*2 =*|ψ _{∞}|*2 =

*−α*

*β,* (α <0).

The diﬀerence of the minimum in the free-energy density between the

su-perconducting (ψ = *ψ _{∞}*) and normal states (ψ = 0), by deﬁnition, is equal
to the opposite of the condensation energy, which is expressed through the

critical thermodynamic magnetic ﬁeld as [5]

*f*_{s}*−f*_{n} =*−α*

2

2β =*−*
*H _{c}*2

8π*.* (1.2)

A material becomes superconductor below the critical temperature*T _{c}*, where

*|ψ|*2 = 0, thus

*α*changes sign at

*T*; expanding the coeﬃcient

_{c}*α*near

*T*yields

_{c}*α(T*) = *α*(T /T_{c}*−*1)*.* (1.3)
With the use of standard variational techniques, by minimizing the free

en-ergy with respect to the order parameter*ψ∗*(**r**) and applying also the Maxwell
equation**j**_{s}=*c/4π*(*∇ ×***h**), the Ginzburg-Landau equations are obtained

*αψ*+*β|ψ|*2*ψ*+ 1
2m*∗*

*i∇ −*
*e∗*

*c* **A**
_{2}

*ψ* = 0, (1.4)

**j**_{s} = *e*
*∗*

*m∗*

*∇ϕ−e*
*∗*

*c* **A**

*|ψ|*2*,* (1.5)

where the second equation gives the supercurrent density**j**_{s}as a diamagnetic

response of the superconductor. The Ginzburg-Landau approach provides a

phenomenological description for temperatures suﬃciently near *T _{c}* and
spa-tial variations of

*ψ*and

**A**which are not too rapid. The equations are gov-erned by the two characteristic lengths for a superconductor: the coherence

length *ξ* and the penetration depth *λ. The meaning of these fundamentals*
parameters can be understood easily from the equations (1.4). In a situation

with no current or ﬁelds, we can restrict the analysis to the real function

*f(r) =ψ(r)/ψ _{∞}*, so the equation becomes
2

2m*∗|α(T*)*|∇*

*1.2. Ginzburg-Landau and London theories*

The linearisation of (1.6) around the superconducting state *f*(r) = 1, leads
to the following equation in terms of *g(r) = 1−f*(r),

*ξ*2*∇*2*g−*2g = 0, *ξ*2 =

2

2m*∗|α(T*)*|* =

*ξ*2(0)

1*−T /T _{c}.* (1.7)
The relation above shows that the order parameter decays with a length of

the order of the coherence length *ξ* which diverges at *T _{c}*, as expected for a
critical phase transition. Similarly, the penetration depth

*λ, is derived from*the second equation for the current density, when a weak ﬁeld is considered.

By approximating the order parameter for a homogeneous superconductor,

*ψ* =*ψ _{∞}* and using Maxwell’s equation,

*∇ ×*

**h**= 4π

**j**

_{s}*/c, we derive*

*∇ ×*(

*∇ ×*

**h**) =

*−*16πe

2

*m∗c*2 *|ψ∞|*

2_{h}_{.}_{(1.8)}

Equation (1.8) shows, by using the relation *∇ ·***h** = 0, that the magnetic

ﬁeld is screened by the diamagnetic currents and decays exponentially in

the superconducting material (the so called Meissner eﬀect). The decaying

length *λ* is deﬁned by

*λ*2(T) = *m*
*∗ _{c}*2

16πe2*|ψ _{∞}*(T)

*|*2 =

*λ*2(0)

1*−T /T _{c},* (1.9)

where the relation (1.3) for the temperature variation is considered. Equation

(1.8), together with (1.9), is written as,

*λ*2*∇ ×*(*∇ ×***h**) +**h**= 0, (1.10)
which can be derived also in the framework of the London theory [42] by

considering the energy functional

*E* =*E*_{0}+ 1
8π

*d*3*r* **h**2 +*λ*2_{L}(*∇ ×***h**)2 *.* (1.11)
Here*E*_{0} is the condensation energy, **h** is the microscopic magnetic ﬁeld, and

*λ*_{L} is the London penetration depth, which is deﬁned by

*λ*2_{L}= *mc*

2

where *n*_{s} is the density of superconducting electrons. The ﬁrst term in the
integral is the magnetic ﬁeld energy, while the second term is the kinetic

energy due to the supercurrents, where the relations **j**_{s} = *n*_{s}*e***v**_{s} and the
Maxwell’s equation *∇ ×***h**= 4π**j**_{s}*/c* have been used.

The London theory is based on the fact that the wavefunction of the

superconducting electrons is constant, with density given by *n*_{s} =*|ψ _{∞}|*2. As
a consequence, the equation above for the supercurrent

**j**

_{s}yields the relation

**j**_{s} =*n*_{s}*e***v**_{s} =*−n*s*e*

2

*mc* **A***,* (1.13)

and, taking the time derivative and using Ampere’s equation, the ﬁrst London

equation is derived

*d***j**_{s}

*dt* =
*n*_{s}*e*2

*m* **E***.* (1.14)

If we vary *E* with respect to **h**, we obtain the second London equation,

which has the same form of (1.10), with*λ*_{L} instead of*λ. Near the regime for*
temperatures closed to *T _{c}*, the two theories must give the same description,
and thus these two lengths coincide,

*λ*

_{L}=

*λ.*

**1.3**

**Type II superconductors**

The ratio of the two characteristic lengths that have been introduced in the

previous sections,

*κ*= *λ*

*ξ,* (1.15)

called the Ginzburg Landau parameter, deﬁnes the distinction between type

I and type II superconductors. One feature for which these two types of

superconducting materials diﬀer, as we have anticipated, is given by the

surface energy of a domain wall between the normal and superconducting

phases; this can be calculated from equations (1.4) and (1.5). The surface

energy is determined in particular by the excess of the Gibbs energy due to

the presence of the superconducting-normal interface over what it would be

*1.3. Type II superconductors*

*H*

*H*

*0*

*T*

*T*

_{c}

_{c}

*H*

### Normal

### state

### state

### Mixed

### state

### Meissner

C1 C2

Figure 1.3: Mean-ﬁeld phase diagram for a type II superconductor. Below

the critical ﬁeld *H _{c}*

_{1}(T), the material in the Meissner-Ochsenfeld phase an external magnetic ﬁeld is totally expelled. Between

*H*

_{c}_{1}(T) and

*H*

_{c}_{2}(T) in the intermediate state, the magnetic ﬁeld penetrates by forming a regular

array of vortices. At *H _{c}*

_{2}(T) the material undergoes a second order phase transition from the mixed to the normal phase.

state. Numerical evaluations have shown that this energy is negative for

values *κ >*1/*√*2, corresponding to type II superconductors [5, 32].

The existence of vortices in type II superconductors was predicted by

Abrikosov [2] in 1957, who solved the Ginzburg-Landau equations for the

case*κ >*1/*√*2 and showed that an equilibrium situation, between two critical
ﬁelds*H _{c}*

_{1}(T) and

*H*

_{c}_{2}(T), is characterised by a regular array of ﬂux tubes. At each site of the lattice, a vortex of supercurrent encircles a quantised amount

of magnetic ﬂux *φ*_{0} =*hc/2e.*

Ginzburg-Landau formalism using the fact that the complex superconducting order

parameter *ψ* must be a single-valued function. As a consequence, the phase
*ϕ* must change by integral multiples of 2π for a closed integral path

*∇ϕ d***s**= 2πn. (1.16)

By considering a loop that encloses a vortex, and integrating for example

through a circular path *γ(R) of radius* *R, it is easy to see that the ﬂuxoid*
*φ*, deﬁned by London [42, 43] as

*φ* =*φ(R) +* 4π
*c*

*γ*(*R*)

*λ*2**j**_{s}*d***s**=

*γ*(*R*)

**A**+ 4πλ

2

*c* **j**s

*·d***s***,* (1.17)

is quantised. Using indeed equations (1.5) and (1.9) for the supercurrent

density **j**_{s} and the penetration depth *λ, one can verify that*
*φ* =*nhc*

*e∗* =*nφ*0*,* (1.18)

with*φ*_{0} =*hc/2e∼*2.07*×*10*−*7 G/cm2. If the radius *R*of the contour is large
enough, *R* *λ, the supercurrent density* **j**_{s} through the loop of integration
decays to zero and the second term on the right of (1.17) can be neglected.

Thus, the total ﬂux trapped by a vortex is also quantised and for *n*= 1,

*φ*=*φ*_{0}*.* (1.19)

At a ﬁnite magnetic ﬁeld *H > H _{c}*

_{1}, the vortices penetrate the system. The array of vortices was later proven to be hexagonal, with the inter-vortex

distance given by [44]

*a*=

4 3

_{1}_{/}_{4}
*φ*_{0}

*B.* (1.20)

As the mean-ﬁeld phase diagram of Fig. 1.3 shows, at the critical ﬁeld*H _{c}*

_{2}(T), there is a second order phase transition from the mixed state with vortices,

called also intermediate state or Schubnikov state, to the normal phase.

*1.4. Magnetic properties of vortices*

the demagnetisation currents, thus the ﬁeld penetrates in the form of quanta

of ﬂux, but the local internal magnetic ﬁeld *B* is less than the applied one.
The density of vortices increases with the magnetic ﬁeld, also according to

(1.20), till the cores of vortices overlap and *a∼ξ* at *H* *∼H _{c}*

_{2}(T).

It is important to stress that the diagram of phase represented in Fig. 1.3

is valid only in a mean ﬁeld approximation, outside of the critical region

in which the ﬁelds ﬂuctuations are important. A measure to estimate the

temperature window in which thermal ﬂuctuations are relevant is given by

the Ginzburg criterion [4]

*|T _{c}−T|< T_{c}Gi,*

*Gi*= 1 2

*T _{c}*

*H*2(0)ξ3(0)

_{c}

*,* (1.21)

where the Ginzburg number *Gi* deﬁned above provides a measure of the
relative size of the minimal condensation energy*H _{c}*2(0)ξ3(0) within a volume
set by the coherence length

*ξ(0) at*

*T*= 0. In this thesis we will consider temperature eﬀects for the phenomena of pattern formation by referring only

to experiments in low-T* _{c}* superconductors, like Nb, for which the Ginzburg
number is very low,

*Gi∼*10

*−*8 and thus, according to (1.21), ﬂuctuations can been neglected [4]. For high-T

*materials, instead, the fundamental Ginzburg parameter is much larger, e.g.*

_{c}*Gi*

*∼*10

*−*2 for YBa

_{2}Cu

_{3}O

_{7}

*, and thermal ﬂuctuations give rise to a richer phase diagram, characterised also by new*

_{−}_{δ}phase transitions, e.g. the melting transition of the vortex lattice. [4] .

**1.4**

**Magnetic properties of vortices**

Since in this thesis we focus on the non-equilibrium patterns of vortices, at

the purpose of understanding their collective behavior and the mutual forces

that act on these interacting strings, we will introduce here the microscopic

magnetic ﬁeld related to a vortex and the interaction energy between two

magnetic ﬂux lines. This is important to understand some issues for this

thesis, for example, why vortices of the same sign tend to repel each other,

the surface tension that plays an important role at the interface with two

diﬀerent phases, e.g. between a normal solid and a liquid [49], cannot be

deﬁned for a domain of vortices, because of the absence of attractive forces.

The form of the magnetic ﬁeld associated with a vortex is needed also to

derive how the currents decay with respect to the distance from the cores.

Moreover, as we will see, while the interaction between vortices is screened

for a slab, in a thin ﬁlm these are long-range. The strength of the currents is

crucial for the formation of the type of dendritic and ﬁnger-like patterns that

we want to analyse, since they have been observed only in thin ﬁlms [11].

**1.4.1**

**Magnetic field of a flux line**

In Sec. 1.2 we have introduced the London theory. This approach is based on

the approximation that neglects the variation of the order parameter and thus

is not capable to describe the vortex core. It is only valid therefore on scales

larger than the coherence length *ξ. However, for type II superconductors*
with a Ginzburg-Landau parameter *κ* 1, deﬁned by (1.15), the London
theory provides a good phenomenological description for the spatial variation

of the internal magnetic ﬁeld.

In the presence of vortices Eq. (1.10) is modiﬁed and a source term on

the right hand side must be included, so that we have

*λ*2*∇ ×*(*∇ ×***h**(**r**)) +**h**(**r**) =*φ*_{0}
*N*

*i*=1

ˆ

**t*** _{i}*(s)δ(

**r**

*−*

**r**

*(s)), (1.22)*

_{i}where *φ*_{0} is the ﬂux quantum and ˆ**t*** _{i}*(s) is the tangent vector along the

*i-th*vortex. Here we assume that the vortices are straight and point along the

ﬁeld direction, which we will take as the **z**-axis. Let us determine ﬁrst the

solution for the microscopic magnetic ﬁeld*h(***r**) for one isolated vortex. Using
*∇ ·***h**= 0, we ﬁnd that Eq. (1.22) becomes

*−λ*2*∇*2+ 1**h**(**r**) = ˆ**z***φ*_{0}*δ(***r**). (1.23)
The solution of this equation is given by the zero order Bessel function

*h(r) =* *φ*0

*1.4. Magnetic properties of vortices*

which has the asymptotic form of a logarithmic behavior at short distances

from the core, and decaying as 1/rexp(*−r/λ) for* *r→ ∞*

*h(r)∼* *φ*0

2πλ2 ln(λ/r), ξ < r *λ,* (1.25)
*h(r)∼* *φ*0

2πλ2

*πλ*
2r*e*

*−r/λ _{, r}*

_{}_{λ.}_{(1.26)}

As we have pointed out, the spatial variation of the magnetic ﬁeld inside the

core can not be considered within the framework of the London theory. The

inferior limit of the relation (1.25) therefore comes from the limitations of

this approach. One should use the Ginzburg Landau formalism to go beyond

the limit *r < ξ.*

**1.4.2**

**Vortex-line Energy**

From the form of the microscopic magnetic ﬁeld**h**, the energy of an isolated

vortex line can be calculated straightforwardly. By considering indeed the

total energy

*E*1 =

1 8π

*h*2 +*λ*2*|∇ ×***h***|*2*,* (1.27)
using the vectorial relation*∇ ·*(**h***×*(*∇ ×***h**)) =*|∇ ×***h***|*2*−***h***· |∇ ×*(*∇ ×***h**)*|*,

and neglecting the core this relation can be written as [5, 6]

*λ*2
8π

**h***×*(*∇ ×***h**)*·d***s***.* (1.28)
Integrating in a loop around the core, the asymptotic logarithmic form that

we have found for the magnetic ﬁeld of a vortex (1.25) yields for*ξ < r* *λ*
*|∇ ×***h***| ∼* *φ*0

2πλ2 1

*r.* (1.29)

Using espression and the relation *h(0)* *∼* *h(ξ), since the magnetic ﬁeld for*
*r < ξ* is approximately constant, the energy of a vortex line is determined as

*E*1 = *φ*
2
0

4πλ2ln
*λ*
*ξ*
= *φ*
2
0

4πλ2 ln*κ,* (1.30)

**1.4.3**

**Interaction between vortices**

Let us consider two interacting vortices. Since the total local magnetic ﬁeld at

a point**r** can be written, in view of the linearity of (1.22), as a superposition

of the two magnetic ﬁelds corresponding to the two vortex cores at a position

**r _{1}** and

**r**respectively,

_{2}*h(*

**r**) =

*h*

_{1}(

**r**) +

*h*

_{2}(

**r**) and substituting into the (1.28), the total magnetic energy can be written as

*E* = 2*E*_{1}+ 2*E*_{12}*.* (1.31)

The ﬁrst term in the expression above is the energy of one vortex lines

calcu-lated in the previous section and derives from the self-interaction due to the

coupling between the magnetic ﬁeld of each vortex and the supercurrent

en-circling the core. The second term expresses instead the energy of interaction

between the two vortices and is given by

*E*12=

**h _{1}**

*×*(

*∇ ×*

**h**)

_{2}*·d*

**s**

_{2}*,*(1.32) where the integration is meant for a loop encircling the vortex at position

**r**. Therefore, by following the same type of calculation of the previous section,

_{2}this is written as

*E*12= _{4π}*φ*0*h(|***r1***−***r2***|*) = *φ*

2 0

8π2*λ*2*K*0

*|***r _{1}**

*−*

**r**

_{2}*|*

*λ*

*,* (1.33)

which shows that the interaction energy between the vortices is proportional

to the magnetic ﬁeld*h(|***r _{1}**

*−*

**r**

_{2}*|*) =

*h(r*

_{12}), so it has a logarithmic dependence for

*ξ*

*r*

_{12}

*< λ*and behaves as as 1/

*√r*

_{12}exp(

*−r*

_{12}

*/λ) for*

*r*

_{12}

*> λ. The*interaction between vortices is

*repulsive*.

The fact that vortices of the same sign repel each other has an important

consequence also for their collective dynamics, on which we want to focus

in this thesis. Unless these interacting strings are in the stable

conﬁgura-tion of an hexagonal array that minimises the free energy of the system or

inhomogeneities prevent their motion, a domain of vortices tends therefore

to expand. On the other hand vortices of opposite charge do attract each

*1.5. The Lorentz force*

opposite sign and the interaction is negative as a consequence of (1.32) and

(1.33), as we will see also in the Chapter 3.

**1.4.4**

**Interactions in a thin film**

As we have seen, at large distances the interaction between vortices is screened

by the supercurrents. This screening eﬀect is reduced in a thin ﬁlm, for

which the thickness *d < λ, and interactions are thus long-range. The *
out-of-equilibrium patterns that we want to describe in this thesis have been

observed mainly in thin ﬁlms, for which the strong interactions play an

im-portant role for the formation of these instabilities. The details of the

deriva-tion of these interacderiva-tions which was done by Pearl, can be found in [47] and

also in [48]. As a result of the analysis the vortex interaction between two

vortices at distance *r*_{12} given by

*E*12(r12) = _{8πΛ}*φ*0 [H0(r12*/Λ)−Y*0(r12*/Λ)],* (1.34)

where *H*_{0} and *Y*_{0} are Hankel functions and the Λ = 2λ2*/d* is an eﬀective
penetration depth for a thin ﬁlm. The asymptotic behavior of this energy is

logarithmic at short distances, like in the case of a slab, for *ξ < r*_{12} Λ
*E*12(r12)*∼* *φ*

2 0

4πΛln

Λ
*r*_{12}

*,* (1.35)

and at large distances, *r*_{12}Λ, decays as
*E*12(r12)*∼* *φ*

2 0

4π2*r*_{12}*.* (1.36)

**1.5**

**The Lorentz force**

From the interaction energy between vortices that we have introduced in the

previous sections one can compute the force that acts on each magnetic ﬂux

line due to the coupling with the supercurrent density**j** of the other vortices.

**f**

**f**

**h**

**h**

**J**

**J**

Figure 1.4: Schematic representation of the origin of the Lorentz force acting

on a vortex, due to the coupling between the local magnetic ﬁeld **h** and a

macroscopic current **J** due to a gradient in the density of vortices.

of the *x-y* plane of a slab one gets
*f*_{2}* _{x}*(

**r**

_{2}) =

*∂F*12

*∂x*_{2} =*−*
*φ*_{0}
4π

*∂h*_{1}(**r**_{2})
*∂x*_{2} =

*φ*_{0}

*c* *j*1*y*(**r**2), (1.37)
where the Maxwell equation *∇ ×***h** = 4π**j***/c* has been used. Extending the
result to the vectorial form, we derive

**f**_{2} =**j _{1}**

*×φ*0

*c* *,* (1.38)

which is the force acting on a vortex at position**r _{2}**, due to the vortex at

**r**. Generalizing the problem for an array of vortices, the total force is given by

_{1}**f** =**J***×* *φ*0

*c* *,* (1.39)

where **J** is the total macroscopic current density acting on a ﬂux line, due

to the presence of the other vortices. Unless the total current vanishes,

a vortex moves thus under the eﬀect of this force, called Lorentz force, or,

*1.6. The dynamics of vortices*

with the hydrodynamical force in a ﬂuid, is represented in Fig. 1.4: in a

non-equilibrium situation, the non-homogeneous vortex density leads to a

gradient in the phase of the superconducting parameter *∇ϕ*at a point in the
space, and, consequentely, for (1.5), to a macroscopic current density **j**_{s} that

is responsible for the motion of the vortices. The Lorentz force in (1.39) is

generated also for any externally imposed transport current.

**1.6**

**The dynamics of vortices**

In this section we will discuss the diﬀerent regimes that characterise the

dynamics of vortices. When vortices move with a velocity **v**, they induce an

electromagnetic ﬁeld [3–6]

**E**=**B***×* **v**

*c,* (1.40)

parallel to**j**, that acts as a resistive voltage, due to the fact that the magnetic

ﬂux trapped in a superconductor decreases. The motion of vortices is thus

accompanied by dissipation, leading to a resistance that destroys the

persis-tent currents. The motion of vortices can be prevented, however, by pinning

forces due to inhomogeneities. Depending on the relative strength of these

forces with respect to the driving Lorenz force, we can distinguish diﬀerent

regimes. For low currents the dynamics is dominated by the so called *creep*

regime, in which vortices hop from one pinning center to an other. This

motion is thermally activated, as we will see in more detail. If the pinning

instead is weak in comparison to the Lorentz force, vortices move with a

steady viscous motion, in which the driving force is balanced by a friction

force. This regime is referred as *ﬂux ﬂow*. The response of the
supercon-ducting material to a macroscopic transport current density **j**, is represented

by the electric ﬁeld-current characteristic, as shown in Fig. 1.5. While for a

*E*

*j*

*j*

### creep

### flow

*E*

*−*

*j*

### ideal

### slope

f

c

*ρ*

Figure 1.5: This ﬁgure represents the form of the electric-ﬁeld current

char-acteristic for the intermediate state of a type II superconductor. For currents

*j* *j _{c}*, the dependence is linear, and the

*E-j*relation is dominated by the ﬂux ﬂow regime, whereas for

*j < j*the

_{c}*E-j*relation is strongly nonlinear and dominated by the creep regime. The idealised

*E-j*characteristic, which is linear above

*j*and equal to zero below

_{c}*j*, is also represented.

_{c}for *j* *≤j _{c}*.

An important consideration to underline for our study in the collective

dynamics of vortices is that, except for the regime of very high ﬁelds and

currents, as a consequence of the strong mutual repulsive interactions

be-tween ﬂux lines, vortices do not move individually, but tend to form bundles

corresponding to several units of ﬂux quantum. This behavior is enhanced

expecially in the creep regime, in which a pinning barrier has to be overcome.

While discussing the dynamics of vortices, we will thus not refer to the

mi-croscopic ﬁeld of a single vortex line, but we will focus on the mami-croscopic

*1.6. The dynamics of vortices*

**1.6.1**

**The flux flow regime**

If pinning is weak, for a vortex that moves with a velocity**v**, the

phenomeno-logical equation that governs the dynamics of vortices is

**F**_{L} =*η***v**=**j***×* *φ*0

*c* ˆ**z***,* (1.41)

where*η* is a viscosity coeﬃcient that we will deﬁne later in this section. The
power which is dissipated in this motion can be expressed in terms of the

viscosity as

*W* =**F**_{L}*·***v**=*ηv*2*.* (1.42)

The simplest approximation for this regime was derived by Bardeen and

Stephen [50], which is based essentially on the two ﬂuid model, according to

which the total electron density can be divided in two parts: the

supercon-ducting component with density *n*_{s} and the normal component with density
*n*_{n}. While for the normal electrons, we can apply Ohm’s law and the relation

**j**_{n} = (n_{n}*e*2*τ*_{n}*/m)***E**, where*τ*_{n} is the relaxation time due to the scattering with
the impurities, for the superconducting component, the approximation based

on the perfect conductivity *τ*_{s} =*∞* is made, like in the London theory [42].
The Bardeen-Stephen model is derived thus by assuming that inside the core

of a vortex, for *r < ξ* there is only the normal component, while outside
the London equation applies. By imposing the continuity of the ﬁeld and

the relation (1.42) for the rate of energy which is dissipated, the viscosity

coeﬃcient *η* is derived

*η* = *φ*0*Hc*2

*ρ*_{n}*c*2 *.* (1.43)

The resistivity for the ﬂux ﬂux regime, which relates the supercurrent density

**j** to the electric ﬁeld **E**, is deﬁned as

*ρ*_{f} = *E*
*j* =

*Bφ*_{0}

*ηc*2 *,* (1.44)

where the expression (1.40) and (1.41) have been used. Combining this last

relation with the result for the Bardeen-Stephen viscosity (1.43), leads to the

rate between the ﬂux ﬂow resistivity *ρ*_{f} and the normal resistivity *ρ*_{n}
*ρ*_{f}

*ρ*_{n} *∼*
*B*
*H _{c}*

_{2}

*∼*

*πξ*2

that equals the ratio between the area occupied by the normal core and the

area per vortex. For *B* *→* *H _{c}*

_{2}the ﬂux ﬂow resistivity tends continuously to the one of a normal metal, as expected, since there is a second order

transition. In reality, as well as this longitudinal viscosity, one can deﬁne a

transversal viscosity given by a Hall eﬀect and the equation for the balance

of the forces is generalised to [3, 4]

*φ*_{0}

*c* **j***×*ˆ**z**=*η***v**+*α*0**v***×*ˆ**z***,* (1.46)
where*α*_{0} *η*for a dirty superconductor with a rather short electronic mean
free path. Usually, the second term due to the transverse Hall eﬀect is thus

neglected in most of type II materials.

In a material characterised by an in-plane anisotropy, as we will see in

Chapter 3, the eﬀective viscous drag coeﬃcient depends on the direction of

propagation of the vortices. More precisely, the mobility deﬁned in (1.41)

becomes a non-diagonal tensor. As a consequence, there is a non-zero

com-ponent of the velocity**v**perpendicular to the driving Lorentz force. In

Chap-ter 3 we will examine the problem of the dynamics of a boundary between

ﬂux and anti-ﬂux and the possible role that the non-collinearity between the

velocity and the force could have on the instability of the front.

**1.6.2**

**The creep regime**

For low current densities, *j* *≤* *j _{c}*, the pinning forces due to inhomogeneities
and defects in the lattice play a relevant role in the dynamics of vortices.

In this regime the current-voltage characteristic is highly nonlinear and

tem-perature dependent. For a driving Lorentz force weaker than the pinning

barrier, the vortex lines move because of thermal activation; their motion is

small but ﬁnite and a weak dissipation is present.

When the magnetic ﬂux penetrates into a superconducting material, the

macroscopic ﬁeld**B**inside the material drops from a ﬁnite value to zero.

*1.6. The dynamics of vortices*

ﬁeld in the ˆ**z** direction and that propagates in the ˆ**x**direction,

*j* = *c*
4π

*dH*
*dx* *≈*

*c*
4π

*dB*

*dx.* (1.47)

where in the last relation the approximation **B** *≈***H** that neglects the

mag-netisation of the sample has been made; this is quite appropriate for a type II

superconducting material with a Ginzburg-Landau parameter*κ*1/*√*2 [5].
Since a Lorentz force given by

**F**_{L}=**j***×* *φ*0

*c* ˆ**z** (1.48)

acts on the vortices, the magnetic ﬂux tends to penetrate further, reducing

the gradient of the magnetic ﬁeld and therefore the current, for (1.47), till

the Lorentz force per unit volume is less than a critical value, determined by

the pinning barrier

*F*_{L} *≤F _{c}.* (1.49)

This situation suggests that ﬂux penetration can be described in terms of a

*critical state*, in which the magnetic ﬁeld enters the superconducting material
with a linear proﬁle with slope 4πj* _{c}/c, according to the Bean model [7].*
This picture, in which the current density

*j*is assumed to be constant and independent on the external magnetic ﬁeld, represents a metastable state,

_{c}which could develop into instabilities like ﬂux jumps and avalanches. From

the general perspective of critical phenomena, this state has been the object

of studies that have focused on the kinetic roughening of the front and the

determination of the scaling behavior of the front ﬂuctuations [46].

As was shown by Kim *et al.*[51], the critical state decays logarithmically
with time at ﬁnite temperatures. This phenomenon was explained with the

creep theory, formulated by Anderson and Kim [52], which is based on the

assumption that vortices jump from one pinning center to an other with a

rate in terms of a thermal activated barrier given by [52]

*R*=*ω*_{0}*e−U*0*/T _{,}*

_{(1.50)}

### a)

### b)

Figure 1.6: Schematic representation of the creep state. a) In the absence

of a net force, vortex bundles jump with unbiased probability to the next

valleys of the pinning potential. b) The presence of a driving force favors

jumps in a “downhill” direction.

coeﬃcient has been omitted here). In the absence of a net force acting on the

vortex bundle, the probability for a jump to a pinning site is independent on

the direction. The situation clearly change when a ﬁnite transport current

makes favorable jumps which are in the “downhill” direction of the driving

force. This situation is represented schematically in Fig. 1.6. The net jump

rate is thus determined by

*R* =*ω*_{0}*e−U*0*/T _{e}*Δ

*U/T*

*−*Δ

_{e}−*U/T*

_{(1.51)}

where ΔU is the work done to move a ﬂux bundle and is therefore

propor-tional to the Lorentz driving force. This leads to a net creep velocity of

*ν* = 2ν_{0}*e−U*0*/T* _{sinh}ΔU

*T* *.* (1.52)

For a large driving force, sinh (ΔU/T) *∼* exp (ΔU/T), the velocity of the

bundle is given by

*1.7. Thermomagnetic instabilities*

Since the barrier *U*(j) vanishes at the critical current *j _{c}*, for currents
suﬃ-ciently close to

*j*,

_{c}*U*(j) can be simpliﬁed as

*U*(j *→j _{c}*)

*≈U*

_{c}1*−* *j*
*j _{c}*

_{α}

*,* (1.54)

where *U _{c}* is the pinning activation barrier [4]. In this thesis we will consider
the Anderson’s original proposal of equation (1.54) with the coeﬃcient

*α*= 1. For conventional low-T

*materials, to which we will restrict in our study while considering the creep regime, the typical values for the activation energy*

_{c}*U*are very large,

_{c}*T /U*

_{c}*≈*10

*−*3 [4, 53].

As we will in the next Chapter, the steepness of the velocity-current

relation, plays a crucial role in the conﬂict between the heat generation and

loss in the material. It is thus very important for the formation of

thermo-magnetic instabilities.

**1.7**

**Thermomagnetic instabilities**

As a consequence of the Joule heating eﬀect induced by the electromagnetic

ﬁeld (1.40), a thermal instability can develop if the amount of heat that

is generated can not be transfered fast enough to the substrate. We will

discuss and underline here the main ideas of the theory of bistability in

superconductors that constitute the starting point to carry our analysis on

ﬁngers patterns in Chapter 2. In this section we will refer in particular to the

reviews of [8, 9]. The Joule self-heating eﬀect in type II superconductors, is

given by the coupling of the electromagnetic ﬁeld**E**in (1.40) and the current

density **j**. By indicating with *Q(T, j) the power density which is dissipated,*
we have

*Q(T, j) =E(T, j)j.* (1.55)
For a thin ﬁlm of thickness *d, in contact with a substrate that is kept at the*
bottom at a ﬁxed temperature *T*_{0}, in the heat balance we take into account
also the amount of energy that is transfered to the substrate; this is given by

*W*(T) = *h*

where*h*is the heat transfer coeﬃcient of the substrate. Equation (1.56) holds
if the temperature change along the thickness of the ﬁlm can be ignored, [8]

*d* *d*_{c}*∼* *K*

*h,* (1.57)

where*K* is the thermal conductivity of the ﬁlm. By considering the diﬀerent
contributions in the equation for the temperature and neglecting the heat

diﬀusion, we derive

*C∂T*

*∂t* =*Q(T, j)−W*(T), (1.58)
where *C* is the heat capacitance of the ﬁlm. The condition of steady-state
balance for a ﬁxed current density**j**is satisﬁed for a temperature*T* such that
*Q(T, j) =W*(T). (1.59)
Linearising (1.58) around the stable point, with respect to small

perturba-tions of the temperature ﬁeld, leads to the stability criterion
*∂W*

*∂T* *>*
*∂Q*

*∂T* *.* (1.60)

As the graﬁc solution of Fig. 1.7 shows, for a steep enough current-voltage

characteristic, the curve that represents the heat generated*Q(T, j) intersects*
the curve corresponding to the heat loss *W*(T) in three points, for current
density *j* in a certain range*j _{∗}*

*< j < j∗*. The states corresponding to

*T*

_{1}and

*T*

_{3}are stable, whereas the one at

*T*

_{2}is unstable, according to the relation (1.60). In order to understand better the conditions in which a thermal

instability can develop, let us consider the idealised *E-j* characteristic, that
we have explained in Sec. 1.6, so that

*E* =*ρ*_{f}(j *−j _{c}*(T)), (j > j

*(T)), (1.61) where*

_{c}*ρ*

_{f}is the ﬂux ﬂow resistivity. Therefore, by indicating with

*T∗*the temperature at which

*j*=

*j*

_{0}(T

*∗*),

*Q(T, j) has the form of a stepped function,*given by the following set of equations

*1.7. Thermomagnetic instabilities*

*Q* (*j*)

*Q* (*j*_{*})

*Q* (*j* )

*T*
*T*_{3}

*T*_{2}

*W*

1 0

*T* *T*

*

Figure 1.7: Graﬁc solution of the heat balance. For a current density in

a certain interval *j _{∗}*

*< j < j∗*, the curves that represent the heat generated

*Q(T, j) and the heat loss to the substrate intersect in three points. The states*corresponding to

*T*

_{1}and

*T*

_{3}are stable, whereas the one at

*T*

_{2}is unstable.

where the last relation follows from the *E-j* relation for a normal metal. By
using the condition of steady state (1.59) and expressing it in the

dimension-less form, with *θ*= (T *−T*_{0})/(T_{c}−T_{0}) and*i*=*j/j*_{0},*j*_{0} =*j _{c}*(T

_{0}), we ﬁnd two intersection points for

*W*(θ) and

*Q(θ)*

*θ*_{2}(i) = *αi(i−*1)

1*−αi* *,* *θ*3(i) =*αi*

2_{,}_{(1.65)}

where we have considered a linear temperature dependence of the critical

current with respect to the dimensionless variables as*j _{c}*(θ) =

*j*

_{0}(1

*−θ). The*dimensionless parameter

*α, deﬁned also as Stekly parameter, is equal to the*ratio between the heat generated for

*j*=

*j*

_{0},

*ρ*

_{f}

*j*

_{0}2 and the heat transfered to the substrate, (T

_{c}*−T*

_{0})h/d

*α*= *ρ*f*j*

2
0*d*

*h(T _{c}−T*

_{0})

*.*(1.66)

*mag-Q*(*j*)

*Q*(*j* )

*W*
*Q*

a)

2 3

2 3

b)

*W*

( )

1− *i*
*j’*

*θ*

*θ*

*θ*

*θ*

*θ*

*θ*

Figure 1.8: Graphic solution of the heat balance for an idealised

current-voltage characteristic in two cases a) for *j > j*_{0} and *α <*1 b) for *j < j*_{0} and
*α >*1.

netic ﬁeld *B* and thus on its spatial variations in the sample. However, here
and in the model that we will develop in Chapter 2 we will consider a

con-stant magnetisation and neglect therefore spatial dependences of the critical

current. Therefore we consider *α* as a constant. Our approximation is
jus-tiﬁed by the fact that an almost constant induction was measured inside

ﬁnger-like and dendritic patterns in the experiments of [11, 12]. Depending

on the relative strength between *j* and *j*_{0}, we have two diﬀerent cases for the
existence of *θ*_{2}: for *j > j*_{0} and *α <*1, or *j < j*_{0} and *α >*1. This situation is
represented schematically in Fig. 1.8, which shows that a thermal instability

due to self-heating can develop only in the second case. The intersection*θ*_{2},
for the superconducting state, corresponding to (1.65) is a stable point for

the ﬁrst case, and unstable point for the second case.

By substituting (1.65) in (1.61), one ﬁnds

*j* = *j*0+*ρ*
*−*1

f *E*

1 +*αE/ρ*_{f}*j*_{0}*,* (1.67)

which shows that the conductivity is decreased due to self-heating. Moreover,

*1.8. Out-of-equilibrium vortex patterns*

the conductivity

*σ(E) =* *∂j*

*∂E* = (1*−α)ρ*
*−*1

f (1.68)

is obtained. Therefore, from (1.68), one can easily see that *σ(E) becomes*
negative for *α >*1. This clearly points out a thermal instability. For *j < j*_{0},
and *α >*1 therefore, self-heating is relevant.

Moreover, a thermal bistability develops for a certain range of current

densities *j*_{m}*< j < j*_{0}, for which the heat balance is satisﬁed in three points,
like represented in Fig. 1.7. This is derived by imposing the heat balance

*ρ*_{f}*j*_{m}2 = (T_{c}*−T*_{0})h(T* _{c}*)/d,

*j*

_{m}as

*j*

_{m}=

*α−*1

*/*2

*j*

_{0}. As it follows from (1.66), the parameter

*α*decreases with the temperature; as a consequence the thermal instability is observed in a certain window

*T*

_{c}*−*ΔT < T

_{0}

*< T*, outside of which

_{c}*α <*1 and self-heating is negligibly small [8]. By considering for example a temperature dependence of the critical pinning current density of

the type *j _{c}*(T) =

*j*

_{0}(1

*−T /T*), and substituting it in (1.66), the interval ΔT is estimated as

_{c}ΔT
*T _{c}* =

*hT _{c}*

*ρ*_{f}*dj*_{0}2*.* (1.69)

The facts that the dendritic and ﬁnger-shape patterns that we will analyse are

observed in a certain temperature window and that the magnetic distribution

does not extrinsically depend on the inhomogeneities of the sample, support

the interpretation of this phenomenon in terms of this bistable character due

to the Joule self-heating eﬀect.

**1.8**

**Out-of-equilibrium vortex patterns**

In the study of fronts in type II superconductors, in this thesis, we will

con-centrate in particular on two diﬀerent examples of dynamical instabilities:

ﬁnger-like patterns and turbulence at the boundary between ﬂux and

anti-ﬂux. By using a high-resolution magneto-optical technique, the development

of an initially ﬂat front into ﬁnger-like or dendritic patterns was ﬁrst

Figure 1.9: On the left: magnetic ﬂux distribution of a Nb thin ﬁlm of

thickness 0.5 *μm after zero-ﬁeld cooling and for a magnetic ﬁeld of 40 mT*
and diﬀerent temperatures. The critical temperature is *T _{c}*

*∼*9.2K. On the right: ﬁnger-like patterns in a 0.5

*μm ﬁlm of Nb atT*= 4.2 K and a ﬁeld of 6.8 mT. After [14].

placing a magneto-optical thin ﬁlm near a superconducting material and

us-ing polarised light to measure the local magnetic ﬁeld. The nucleation of

these patterns ranges from one-dimensional structures at 3-4 K, that we will

indicate with “ﬁngers”, to a more complex magnetic ﬂux distribution with

“sea-weed-like” branches, which are referred as “dendrites”, at 6-7 K. These

instabilities were found only in a temperature window, outside which the

magnetic ﬂux penetrates uniformly; in these experiments, in particular, they

were observed between*T /T _{c}*

*∼*0.35 and

*T /T*

_{c}*∼*0.65, for a critical tempera-ture

*T*= 9.2 K. Dendrites nucleate and propagate very fast, independently of the rate at which the external magnetic ﬁeld is increased, and the velocity

_{c}of propagation is sometimes not even measurable with the resolution of a

standard magneto-optical technique. Finger-like patterns were studied also

in detail by Welling et al. [13, 14]. In Fig. 1.9, taken from the experiments,

*1.8. Out-of-equilibrium vortex patterns*

Figure 1.10: a) Overlapping images related to diﬀerent experiments in the

same sample at 4.2 K and 20 mT, which show that the instability does

not depend trivially on defects and inhomogeneities (see for a color version

Physica C **411**, 11 (2004)). b) At 6.7 K the magnetic ﬂux distribution

presents a more complex structure with dendrites. After [14].

ﬁlm of 0.5*μm on a sapphire substrate after zero-ﬁeld cooling and for a *
mag-netic ﬁeld of 40 mT and diﬀerent temperatures. The white areas represent

the Shubnikov mixed state with vortices, while the dark area stand for the

superconducting Meissner state.

As one can observe, with increasing the temperature, the structure of the

domains of vortices becomes more irregular, presenting the morphology of

dendritic patterns. The image on the right reproduces instead instantaneous

bursts of magnetic ﬂux with the well deﬁned ﬁnger-like shapes at 4.2 K.

Fig. 1.10 represents overlapping images related to diﬀerent experiments

in the same sample at 4.2 K and 20 mT. The image clearly shows that the

instability is intrinsic and does not depend trivially on defects and

inhomo-geneities. At 6.7 K the magnetic ﬂux distribution presents a more complex

structure with dendrites.

Figure 1.11: “Turbulent” behavior observed at the boundaries between

vor-tices and antivorvor-tices in a YBa_{2}Cu_{3}O_{7}* _{−}_{δ}* single crystal at a temperature of
65 K. The sequence shows the time development after a) 10 s, b) 20 s, c) 30

s, d) 40 s, e) 60 s, f) 90 s and g) 150 s. After [24].

patterns can be studied in terms of an intrinsic instability due to the

over-heating of the sample. The thermo-magnetic nature of these instabilities due

to the competition between the Joule heat released and the the relaxation

to the substrate, that we have described in the previous section, has been

proposed in [19–21]. We will show the importance of this mechanism in

the selection of the patterns characteristics like the shape and the width of

the ﬁngers. In our analysis we will consider the approximation in which the

density of vortices inside the domain is constant and we will therefore assume

a non-zero current density only at the edge of the domain of vortices.

As we will also discuss in Chapter 2 these pattern have been shown to

reproduce the temperature distribution of the sample. The interpretation

that has been suggested for these phenomena [19, 20] is that the dissipation

induced by the motion of vortices leads to an increase of the ﬁlm

temper-ature and thus to a lower pinning barrier and an enhanced mobility. As a

*1.8. Out-of-equilibrium vortex patterns*

to avalanches. The condition of thermo-magnetic bistability that we have

discussed in the previous section is crucial for the development of this

mech-anism. In this thesis we will support and conﬁrm this argument by proposing

a model in which the shape of the vortex ﬁngers is strictly dependent on the

temperature of the pattern.

While it is now generally accepted that the formation of ﬁnger-like and

dendritic patterns is of thermo-magnetic origin, in the case which has been

referred to as turbulent behavior of a front between vortices and antivortices,

the origin of the instability is not well understood. Fig. 1.11 represents the

“turbulent” state observed in a sample of YBa_{2}Cu_{3}O_{7}* _{−}_{δ}* crystal. After
apply-ing a reversed ﬁeld to a previously remanent state, a new domain of

antivor-tices entering the sample from the edges annihilates with the already existing

state with vortices. The boundary between the ﬂux and anti-ﬂux exhibits an

irregular “meandering” behavior, in a temperature window between 47 and

80 K. The image represents the time development of this instability [24]. We

will discuss in Chapter 3 this type of behavior and examine if the in-plane

**Chapter 2**

**Finger-like patterns**

In this chapter we will focus on the ﬁnger-like patterns that characterise the

magnetic ﬂux distribution in a Nb thin ﬁlm [13] and that are represented in

Fig. 1.9 and Fig. 1.10. These ﬁngers of vortices, that we have described in

Chapter 1, have a well deﬁned shape and a characteristic width that varies

between 20-50*μm. The physical mechanism that underlies the development*
of an instability of a ﬂat front between the vortex and the superconducting

states into these narrow structures has been studied in recent theoretical

models [19–21]. However, while in these earlier work the thermo-magnetic

origin of the instability has been pointed out, the remarkably well deﬁned

shape of the ﬁngers could not be obtained explicitly. In this chapter we will

concentrate particularly on this growth form.

**2.1**

**The sharp interface limit**

A detailed analysis for the shape of the ﬁngers requires a more tractable

mathematical model than the ones proposed previously. In particular, since

we are interested in the dynamics of the front between two phases, we need

to reduce the problem to an interfacial description, in order to determine an

explicit equation for the pattern curvature. The formulation of a local growth

### V

### S

### O

**j**

**j**

*s*

**t**

**n**

**z**

**r**

( *s*

(
*θ*

Figure 2.1: Schematic representation of a local growth model for an interface

between a vortex and a superconducting phase (which are denoted by*V* and
*S* respectively). Each point at the interface, that corresponds to the local
arclength *s, is deﬁned by the angle* *θ* between the normal vector **n** and a
ﬁxed direction **z** in the plane and the distance *r* from a ﬁxed origin (O).

and the characteristics of the pattern in its essential features, without loosing

the required accuracy for a realistic physical description.

Let us consider the general problem of a front propagation between two

phases, in which we can deﬁne a continuous order parameter that vanishes

in a relatively thin transition zone. In an interfacial formulation, or moving

boundary approximation, the dynamics of the front is described by some

boundary conditions for the physics at the interface, without taking into

account explicitly the way in which the order parameter changes from one

state to an other. This method is appropriate if the thickness of the interfacial

region can be neglected in comparison to the typical length scale of the

patterns. If this requirement is satisﬁed, the domain wall between the two